Toward Fundamental Understanding of Peculiar Magnesium
Segregation during Welding of Advanced High-Strength Aluminum
Andrea J. Peer
Advisors: Tyler Borchers and Wei Zhang, The Ohio State University
Motivation Results & Discussion
Questions to be Answered & Approach
• Advanced lightweight materials are crucial for the automotive industry to meet the
increasingly strict vehicle fuel-efficiency standards.
• Lightweight vehicles = better fuel economy
• High-strength aluminum has a high specific strength (strength-to-weight ratio) among various
• The use of high-strength aluminum can increase the fuel efficiency but joining
procedures must be evaluated due to material weldability issues.
• GMAW of 7xxx series high strength aluminum alloys with AA 5356 (Al-Mg) filler wire
can be susceptible to stress corrosion cracking (SCC) when placed under a tensile
stress in a corrosive environment.
• The three factors in the diagram below are needed for SCC to occur.
• Previous work confirmed that failure does not occur without all three factors present.
• SCC initiation takes place at the weld toe and then propagates through the base material under the
• Goal: Develop a mechanistic understanding of Mg enrichment /
segregation and the subsequent formation of T-phase to the weld toe.
•A fundamental understanding of Mg segregation can provide the scientific
•Optimizing welding processes
•Enhancing material use
•This will be beneficial for the widespread use of aluminum alloys for vehicle
light-weighting and fuel efficiency.
Necessary Factors for SCC
• The root cause for stress corrosion crack initiation has been correlated to a Mg-rich
region at the weld toe.
• T (tau) phase [Mg32(Al, Zn)49] continuously precipitates along the grain boundaries in the weld toe.
• This localized segregation is peculiar, as it is unseen throughout the bulk of the weld metal.
• Furnace Melting:
• Determine the segregation characteristics of Mg upon
solidifying from above and below the Mg vaporization point.
• Two temperature levels were tested:
• 900˚C, which is above liquidus (630˚C) but below
vaporization (1107˚C) Mg remains in liquid solution
• 1193 ˚C, which is above vaporization Mg
vaporizes at this temperature
• Geometry Alteration:
• Geometry Alteration:
• Formation of Mg-rich weld toe upon re-melting
• Mg-rich weld toe forms during welding and is not due to initial material mixing.
• Geometry Alteration
• Furnace Melting
Lap Joint Re-melt weld toe at 200x
•Material to the right of the interface formed due to
wetting during re-melt
•Hypothesized wetting flow characteristics are shown by
green arrows in micrograph A
• Mg enrichment along wetting interface (Figure A & 2)
• Test 1: 900˚C
• Mg segregation characteristics viewed
upon heating into liquidus
• From EDS images (Figures E & F):
• Center of grain solidifies first
• FCC Aluminum
• Two phases present at the grain
• Mg-rich phase
• Mg segregating to grain
• Si-rich phase
• Si diffusing from porcelain
• Minimal Zn present in sample
• The weld toe is machined away to remove the Mg-rich region
• Remaining weld material is re-melted with AC current (GTAW)
Stress Corrosion Cracking Resistance
• Test 2: 1193˚C
• Mg segregation characteristics viewed upon
heating above vaporization temperature
• From EDS images (Figures G & H):
• Many more precipitates form
• Si-rich phase
• Si diffusing into sample from
• Fe-rich phase
• Small amount of iron in sample
• Possible contamination
• Negligible Mg present
• Negligible Zn present
• From EDS Images (Figures I & J):
• MgO oxide forms with porcelain crucible
• Mg has high affinity for O
• Figure I shows MgO in Test 1 (900°C)
• Figure J shows MgO in Test 2 (1193°C)
• Figures i and j show oxygen presence in
• Sample etched with Kellers etchant
Figure B & C
Al Mg Zn
B • White “stringer”
phase rich in Mg
in Figure B can be
seen along entire
interface in Fig. 2
•Figure C is EDS Imaging of Figure B
•Figure F is EDS imaging of Figure E •Figure H is EDS imaging of Figure G
 "Black Deposit on and besides the Weld." MIG WELD GmbH International. MIG WELD GmbH International. Web. 21 May
• Repeat Test 1 (i.e., Geometry Alteration) in a 100% Ar-filled chamber to minimize the
formation of MgO during welding.
• MgO Presence
• Figure K show EDS image of the weld toe region
after re-melting in the 100% Ar-filled chamber.
•Surprisingly, Mg enrichment in the re-melted toe
is much less prevalent that in the baseline re-
melting test (Figure C).
• Further characterization using electron microscopes
is ongoing to understand the phase(s) in the re-melt.
• The preliminary results indicate that the MgO
presence during welding is a potential factor for the
formation of Mg-rich weld toe.
• MgO Presence:
• When welding in 100% Ar-filled chamber, Mg
segregation to the weld toe is much less severe.
• Furnace Melting:
• Mg does vaporize above 1107°C
• Mg has a high affinity for O
• MgO forms when oxygen is present
• MgO is favored over Mg in solution
• Determine if the Mg-rich region reappears upon
removal and re-melt.
• Establish if the phenomena occurs during primary
material mixing or due to characteristics under the arc.
Research Supported by Honda R&D Americas Inc.
through CIMJSEA at The Ohio State University
1. If the Mg-rich weld toe is removed from the original weld, could
the segregation re-occur in a subsequent re-melting?
2. Mg is likely to evaporate from the hot region of weld pool
surface as it has a low vaporization temperature. Any effect?
3. MgO, in the form of black deposit on
and beside the weld, is commonly
observed in welding of Mg-bearing
aluminum . Any effect?
Although they did not reveal the results originally
designed due to porcelain crucible
“contamination”, the furnace melting tests did
show the high affinity of Mg for O.
This research points to the
commonly observed MgO as
a potential factor for
formation of Mg-rich weld
toe. Future study is planned
to understand the effect of
MgO on enrichment.